Different physical properties of carbon allotropes (Ma et al., 2010)
Since the first discovery of carbon nanotubes (CNTs) in 1991, CNTs have generated enormous research activities in many areas of science and engineering due to their combined exceptional mechanical, thermal and electronic properties. These properties make nanotubes ideal, not only for a wide range of applications but also as a test-bed for fundamental scientific studies (Baughman et al., 2002). They can be described as a graphite sheet rolled up into a nanoscale tube. Two structural forms of CNTs exist: single-walled (SWCNTs) and multi-walled (MWCNTs) nanotubes. CNT lengths can be as short as a few hundred nanometers or as long as several micrometers. SWCNT have diameters between 1 and 10 nm and normally capped ends. In contrast, MWCNT diameters range from 5 to a few hundred nanometers because their structure consists of many concentric cylinders held together by van der Waals forces. CNTs are synthesized in a variety of ways, such as arc discharge, laser ablation, high pressure carbon monoxide (HiPCO), and chemical vapor deposition (CVD) (Dresselhaus, 1997). CNTs exhibit excellent mechanical, electrical, thermal and magnetic properties. The exact magnitudes of these properties depend on the diameter and chirality of the nanotubes and whether their structure is single- or multi-walled. Fig. 1 shows a segment of a single graphene plane that can be transformed into a carbon nanotube by rolling up into a cylinder. To describe this structure, a chiral vector is defined as
The basic structure of CNTs is comprised of
Other excellent physical properties of CNTs have also attracted much attention. The properties are summarized and compared with other carbon allotropes in Table 1. Because of their unique properties, many promising applications and potential practical applications have been reported, such as field emission materials, catalyst support, electronic devices, nanotweezers, reinforcements in high performance composites, supercapacitors, hydrogen storage and high sensitivity sensors and actuators. These are just a few possibilities that are currently being explored. As research continues, new applications will also develop (Dresselhaus et al., 2004).
|Specific gravity (g cm-3)||1.9-2.3||3.5||1.7||0.8||1.8|
|Electrical conductivity (S cm-1)||4000||10-2-10-15||10-5||102-106||103-105|
|Electron mobility (cm2 V-1 s-1)||2.0 QUOTE||1800||0.5||~105||104-105|
|Thermal conductivity (W m-1K-1)||298||900-2320||0.4||6000||2000|
|Coefficient of thermal expansion (K-1)||-1 QUOTE||(1-3) QUOTE||6.2 QUOTE||~0||~0|
|Thermal stability (in air) (K)||450-650||<600||600||"/600||"/600|
2. Processing of carbon nanotube composites
CNT-based polymer composite materials are being utilized in an increasing number of applications including automotive, aerospace, defence, sporting goods and infrastructure sectors. This is due to their high durability, high strength, light weight, design and process flexibility,
Especially electrically conductive CNT-polymer composites are used in anti-static packaging applications, as well as in specialized components in the electronics, automotive, and aerospace sectors. The incorporation of conductive filler particles into an insulating polymer matrix leads to bulk conductivities at least exceeding the anti-static limit of 10-6 S/m. Common conductive fillers are metallic or graphitic particles in any shape (spherical, platelet-like or fibrous) and size. However, the incorporation of CNTs allows lower percolation threshold compared to other conductive fillers (Fig. 2). The use of CNTs as a conductive filler in polymers is their biggest current application (Bal & Samal, 2007).
The effective utilization of CNTs in composite applications depends strongly on the ability to homogeneously disperse them throughout the matrix without destroying their integrity. Therefore, it has become clear that the issues of dispersion, alignment, and stress transfer are crucial, and often problematic at nanoscale. However, in order to be able to utilize CNTs and their properties in real-world applications, CNT-based nanocompsites provide a pathway to realize the properties of these fascinating nanostructures at macroscopic levels by bridging over a range of length scales.
2.1. Carbon nanotube dispersion
The potential of using nanotubes as a constituent of polymer composites has not been presently realized mainly because of the difficulties associated with dispersion and processing. High aspect ratio, combined with high flexibility, increase the possibility of nanotube entanglement and close packing. The low dispersity comes from the tendency of pristine nanotubes to assemble into bundles or ropes like shown in Fig. 3 (Thess et al., 1996). Thus, a significant challenge in developing high-performance CNT-polymer composites is to introduce the individual CNTs in a polymer matrix in order to achieve better dispersion and alignment and strong interfacial interactions, to improve the load and electron transfer across the CNT-polymer matrix interfaces.
2.1.1. Mechanical dispersion of carbon nanotubes
Although in most cases, it is very difficult to get a homogeneous dispersion of the CNTs in the polymeric matrix, ultrasonication is a very effective method of dispersion and de-agglomeration of CNTs, as ultrasonic waves of high-intensity ultrasound generates cavitation in liquids. There are two major methods for delivering ultrasonic energy into liquids, the ultrasonic bath (Fig. 4. (a)) and the ultrasonic horn (Fig. 4(b)). Ultrasonication disperses solids primarily through a microbubble nucleation and collapse sequence. The ultrasonication bath has a higher frequency (40–50 kHz) than cell dismembrator horns (25 kHz). Ultrasonication of fluids leads to three physical mechanisms: cavitation of the fluid, localized heating, and the formation of free radicals. Cavitation, the formation and implosion of bubbles, can cause dispersion (Lu et al., 1996).
However, ultrasonication affects not only CNT dispersion but also its length and diameter (Fig. 4 (c)). After reducing their lengths during ultrasonication, SWCNTs rearrange into superropes. These superropes have diameters more than 20 times the initial bundle diameter (Shelimova et al., 1998). In MWCNTS, ultrasonication creates expansion and peeling or fractionation of MWCNT graphene layers. The destruction of MWCNTs seems to initiate on the external layers and travel towards the center. It has been reported that the nanotube layers seem quite independent, so MWCNTs would not only get shorter, but actually thinner with time (Lu et al., 1996). There have been attempts to develop less destructive ultrasonication methods. One example is ultrasonication with diamond crystals, a method that reportedly destroys the SWCNT bundles but not the tubes. Raman spectra showed typical SWCNT peaks even after 10 hours of treatment with this method (Haluska et al., 2001).
Ball milling is a method that is usually used to grind bulk materials into fine powder. During milling, a high pressure is generated locally due to the collision between the rigid balls in a sealed container (Fig. 5). Cascading effect of balls reduces the size of material to fine powder. Balls are usually made by ceramic, flint pebbles and stainless steel.
Ball milling has been successfully applied to CNT dispersion into polymer matrices. To obtain narrow length and diameter distributions of CNTs and to open the nanotubes for improved sorption capacity for gases, ball-milling is a very useful method (Awasthi et al., 2004). However, it has also been observed that a large amount of amorphous carbon is created which clearly indicates that the tubes are damaged in different ways and that ball-milling is a destructive method (Jia et al., 1999).
Calendering (Three-Roll mill)
Calendering, also commonly known as three-roll-milling (Fig. 5 (a)) is a dispersion technique that employs both shear flow and extensional flow created by rotating rolls of different speed to mix and disperse CNTs or other nanoscale fillers into polymers or other viscous matrixes. The first and third rollers (usually called the feed and apron rolls, respectively) in Fig. 5 (b) rotate in the same direction while the center roller rotates in the opposite direction. In order to create high shear rates, angular velocity of the center roll must be higher than that of feed roll (ω2 > ω1). As the resin suspension is fed into the narrow gap (
One of the unique advantages of this technique is that the gap width between the rollers can be mechanically or hydraulically adjusted and maintained, thus it is easy to obtain a controllable and narrow size distribution of particles in viscous materials. In some operations, the width of gaps can be decreased gradually to achieve the desired level of particle dispersion (Viswanathan et al., 2006). A typical calendering machine and its principle are shown schematically in Fig. 5. The employment of a calender to disperse CNTs in a polymer matrix has become a very promising approach to achieve relatively good CNT dispersion according to some recent reports (Thostenson & Chou, 2006a).
However, the fed material should be in a viscous state when mixed with CNTs, thus this tool may not be applied to disperse CNTs into thermoplastic matrices, such as polyethylene, polypropylene and polystyrene. In contrast, CNTs can be conveniently dispersed into the liquid monomer or oligomer of thermosetting matrices, and nanocomposites can be obtained via
Extrusion (Melt Compounding)
Extrusion is a popular technique used to disperse CNTs into solid polymers, including most thermoplastics, where thermoplastic pellets mixed with CNTs are fed into the extruder hopper. In particular, twin-screw extruders (Fig. 7. (a)) are used extensively for CNT-polymer mixing and compounding. The modular design of twin-screw extruder allows this operation to be designed specifically for the formulation being processed (Fig 7. (b)) (Bauhofer & Kovacs, 2009). For example, the two screws may be co-rotating or counter-rotating, intermeshing or non-intermeshing. In addition, the configurations of twin-screw extruders themselves may be varied using forward conveying elements, reverse conveying elements, kneading blocks, and other designs in order to achieve each CNT-polymer mixing characteristics. This technique is particularly useful in producing CNT-polymer composites with high filler contents. However, care must be taken to prevent CNT damages due to excessive shear stresses imposed during the extrusion process.
Polymer melt compounding is useful, especially in industry because it does not demand additional processes. However, the melt compounding studied and optimized so far has been mostly focused on micro-compounders at lab-scale. Scale-up of these techniques are not just a matter of size but also a matter of different rheological and thermodynamical issues (Oh & Hong, 2010).
2.1.2. Dispersion of carbon nanotube based on functionalizationCovalent Functionalization
Functionalization of CNTs is an effective way to minimize nanotube interaction, which helps to better disperse and stabilize the CNTs within a solvent or polymer matrix. There are several approaches for functionalization of CNTs, including covalent and non-covalent functionalizations.
In the case of covalent functionalization, the structure of CNTs is disrupted by changing
Carboxylic functionalized CNT surfaces can be further used to chemically attach other small molecules or macromolecules through the reaction of the oxidation-induced functional groups. One of the common chemical reactions with acid functionalized CNT is the amidization, in which amide bond between amine group moieties is formed. One example is the use of amino-functionalized MWCNTs in epoxy systems to yield improved mechanical properties (Stevens et al., 2003). The improved mechanical performance in these functionalized systems may reflect both the enhanced dispersion and an improved surface interaction between CNT and polymer matrix. Further improvements in solubility can be achieved by fluorination, again leading to improvements in both the stiffness and strength, with the addition of 1 wt.% of oxidized and fluorinated SWCNTs. Also, it has been established that the electrical properties of MWCNTs change after fluorination, leading to a wide range of electrical structures, from insulating over to semiconducting and metallic-like behavior (Seifert et al., 2000).
The chemically functionalized CNTs can produce strong interfacial bonds with many polymers, allowing CNT-based nanocomposites to possess high mechanical and functional properties.
A non-covalent method used to modify CNT surface is popular functionalization method since it does not compromise the physical properties of CNTs. The electrostatic repulsion provided by adsorbed surfactants stabilizes the nanotubes against the strong van der Waals interactions between the nanotubes, hence preventing agglomeration. This repulsive and attractive force balance creates a thermodynamically stable dispersion, which results in separation of CNTs from the bundles into individual nanotubes. Anionic surfactants, such as sodium dodecylsulfate (SDS) and sodium dodecylbenzene sulfonate (NaDDBS), are commonly used to disperse CNT aggregation in polar media. The interaction between the surfactants and the CNTs depends on the nature of the surfactants, such as its alkyl chain length, headgroup size, and charge (Fig. 9) (Ma et al., 2010).
The physical interaction of polymers with CNTs to make specific formation can be explained by the ‘wrapping’ mechanism which is π-stacking interactions between the polymer and the nanotube surface. Usually, wrapping polymer consists of aromatic groups on main chain or substitutional groups. For example, polyvinyl pyrrolidone (PVP) or polystyrene sulfonate (PSS) wrapped CNT shows improved dispersity and electrical properties compared to those of the individual components (Cheng et al., 2008).
Small angle neutron scattering studies demonstrated a non-wrapping conformation of polymers in CNT dispersions. In these cases, different structures and compositions of copolymers efficiently act as stabilizers. The suggested mechanism of non-wrapping is that one of the blocks in block copolymers adsorbed to the nanotubes surfaces and another solvophilic blocks act as a steric barrier that leads to the formation of stable dispersions of individual CNTs above a threshold concentration of the polymer. A study of the stabilization effect produced by different diblock or multiblock copolymers led to the conclusion that selective interaction of the different blocks with solvent is essential in order to obtain stable colloidal dispersions of CNTs (Nativ-Roth et al., 2007).
2.2. Control of carbon nanotube orientation
Similar to conventional fiber-reinforced composites, both mechanical properties and functional properties, such as electrical, thermal and optical properties of CNT-polymer composites are directly related to the alignment direction of CNTs in the matrix. Recently, this topic has drawn much attention due to the advance in nanocomposite processing techniques and the limitaions of randomly oriented, discontinuous nanotube composites.
2.2.1. Orientation of carbon nanotube by yarn formation
Recent advances in fabrication of CNTs allow to grow up to several millimeters in length, and these CNTs are possibly aligned to continuous macroscopic SWCNT fibers (Fig. 10). This provides an opportunity for fabricating continuous nanotube reinforced composites.
It has been reported that free-standing arrays of millimeter long, vertically aligned multiwalled nanotubes exhibit supercompressibility, outstanding fatigue resistance, and viscoelastic characteristics. Continuously aligned nanotube reinforced polydimethylsiloxane (PDMS) composite shows remarkably enhanced compressive modulus and strength, anisotropic characteristics, and damping capability (Ci et al., 2008).
2.2.2. Force field orientation
The first method developed to fabricate aligned CNTs in polymer matrix was by ‘‘cutting’’ an CNT-epoxy nanocomposite. This process is simply explained by the nature of rheology in composite media on nanometer scales and flow-induced anisotropy produced by the ‘‘cutting’’ process. The fact that CNTs do not break and are aligned after cutting also suggests that they have excellent mechanical properties along the nanotube direction. However, the orientation of CNTs in CNT-epoxy composite is affected by the cut slice thickness, since the alignment effect is only effective near the slice surface (Ajayan et al., 1994).
A solution approach involved a SWCNT-dispersed surfactant solution (sodium dodecyl sulfate, SDS) injected through a syringe needle into a polyvinyl alcohol (PVA) solution. Because the PVA solution is more viscous than the SWCNT suspension, there is a shear contribution in the flow at the tip of the syringe needle, the flow-induced alignment is maintained by the PVA solution, and SWCNTs are rapidly stuck together as they are injected out from the syringe. By pumping the polymer solution from the bottom, meter-long ribbons are easily drawn, and well-oriented PVA-CNT composite fibers and ribbons are formed by a simple process. It offers a method to align CNTs by a flow field (Vigolo et al., 2000).
The more effective and convinient method in CNT orientation is uniaxially stretching of polymer-CNT composite films. CNT-polymer composite films and fibers produced by any process can be drawn uniaxially showing higher conductivity along the stretched direction than the direction perpendicular to it. Also, the mechanical properties such as elastic modulus and yield strength of composite fibers increased with draw ratio, and CNTs in the composite fibers were better aligned. It is also possible to prepare aligned CNT composite films by extruding the composite melt through a rectangular die and drawing the film prior to cooling. For example, as compared to the drawn polystyrene (PS) film, the tensile strength and modulus of the PS-MWCNT composite films were greater (Thostenson & Chou, 2002).
However, PS-MWCNT composites prepared by spin casting at high speed showed that MWCNTs were aligned in specific angles relative to the radial direction: 45º and 135 º on average. The presence of 2.5 vol.% MWCNTs doubles the tensile modulus and transforms the film from insulating to conducting. It is also noted that the CNTs have higher orientation than the polymer matrix during melt-drawing of the polymer-CNT composites (Bhattachacharyya et al., 2003).
2.2.3. Electric or magnetic field induced orientation
Studies of SWCNT alignment using electric or magnetic fields have usually involved epoxies or polyesters as matrices because of their low viscosity before cure. Under the electric field, it was shown that both AC and DC electric fields can be used to induce the formation of aligned CNT networks spanning the gap between electrodes in contact with the dispersion. With increasing field strength, the quality of these networks and the resulting bulk conductivity of the composite material can be enhanced(Martin et al., 2005). However, at high CNT content, thus high viscosity of molten resin system, the magnetic field-induced alignment of polymeric materials is more effective in CNT alignment. This technique has been the focus of several research efforts, initiated by the first use of high magnetic field to align MWCNTs in a polyester matrix to produce electrically conductive and mechanically anisotropic composites. A high magnetic field is an efficient and direct means to align CNTs. For example, to align MWCNT dispersed in methanol suspension, a magnetic field greater than 7 T is demanded. For the CNT alignment in a polymer, even higher magnetic field would be demanded because of high viscosity. Under a high magnetic field of 10 T, it has been shown that MWCNTs were aligned in the monomer solution during their polymerization and MWCNTs were aligned parallel to the magnetic field inside the polymer matrix (Camponeschi et al., 2007). Recently, magnetic field aligned polycarbonate (PC) and CNT-epoxy composites hae been reported and they suggested that aligning CNTs in polymer matrices can improve mass transport property as well as electrical conduction. It is also viewed that CNTs are better aligned in a PC matrix using magnetic field as compared to an electric field (Abdalla et al., 2010).
2.2.4. Electrospinning induced orientation of carbon nanotube in polymeric nanofiber
Among several approaches to align nanotubes, the electrospinning technique has recently ben used to incorporate CNTs in a polymeric matrix to form composite nanofibers, combining the benefits of nanofibers with the merits of CNTs. Due to the sink flow and the high extension of the electrospun jet, it is expected to align the nanotubes during the electrospinning process, as was also predicted by a mathematical model. However, the distribution and alignment of the nanotubes in the nanofibers are strongly associated with the quality of the nanotube dispersion prepared before addition of the spinnable polymer solution. Generally, well-dispersed MWCNTs were incorporated as individual elements mostly aligned along the nanofiber axis. Conversely, irregular nanotubes were poorly aligned and appeared curled, twisted, and entangled. It is also suggested that the nanofiber diameter, the interaction between the spun polymer and the nanotubes and wetting ability are important factors affecting the alignment and distribution of the nanotubes. This was demonstrated by the difference in the alignment of SWCNTs in polyacrylonitrile (PAN) and polylactic acid (PLA) nanofibers (Ko et al., 2003). More recent work to incorporate SWCNTs into PEO nanofibers by the electrospinning process showed SWCNTs were embedded in PEO in a more regular form since SWCNTs are much smaller and uniform in shape and size, as compared to MWCNTs. On the other hand, their stronger tendency to bundle up into coiled aggregates introduces a pronounced difficulty. Therefore, special attention is given to the dispersion process, which is essential for successful alignment of the nanotubes by the electrospinning process. Structural analysis of the composite nanofibers in terms of the distribution and orientation of both the nanotubes and the polymer matrix has been studied (Salalha et al., 2004).
3. Electrical properties of carbon nanotube composites
CNTs have clearly demonstrated their capability as fillers in conductive polymer composites. Percolation theory predicts that there is a critical concentration at which composites of insulating polymers become electrically conductive. According to the percolation theory, conductivity of composite ( ) can be estimated from the following equation.
|Polymer matrix||CNT type||Maximum filler content (wt.%)||Processing or dispersion method||Maximum electrical
|Percolation threshold (wt/%)||Reference|
|PS||SWCNTs||2||Solution mixing||10-3||0.27||Chang et al., 2006|
|PS||Aligned CNT array||Drop Casting||1330||Peng et al., 2009|
|HDPE||Acid- SWCNTs||6||Extrusion||10-1||~4||Zhang et. al., 2006|
|LDPE||Acid -MWCNTs||10||Ball mill||~2||~1-3||Gorrasi et al., 2007|
|PP||MWCNTs||10.7||Melt mixing||4.6||1.1||Miˇcuˇsík et al., 2009|
|PMMA||SWCNTs||25||Coagulation||10-1||~1||Narayan et al., 2009|
|PMMA||MWCNTs||0.4||Solution mixing||3103||0.003||Kim et al., 2004|
|PMMA||Aligned CNT||-||Drop casting||1250||-||Peng et al., 2009|
|PC||MWCNT||15||Extrusion||20||1-2||Potschke et al., 2002|
|PC||PPE-SWCNTs||10||Solution mixing||4.8102||0.11||Ramasubramaniam et al., 2003|
|Nylon 6||MWCNTs||10||Melt mixing||0.1||2-2.5||Krause et al., 2009|
|Nylon 6,6||MWCNTs||10||Melt mixing||0.1||0.5-1||Krause et al., 2009|
|PDMS||MWCNTs||2.5||Ultrasonica-tion||0.02||1.5||Khosla A & Gray BL, 2009|
|PI||MWCNTs||1.5||3.8310-4||-||Xiaowen et al., 2005|
|PI||Acid- MWCNTs||7||Solution mixing||3.810-6||-||Yuen et al., 2007|
|PU||MWCNTs||27||Solution casting||2103||0.009||Koerner et al., 2005|
|PET||SWCNTs||5||Melt mixing||~1||0.024||Hernandez et al., 2009|
|Epoxy||Aligned SWCNT||5||Solution casting||~10-5||0.5||Qing et al., 2008|
|Epoxy||Silane-MWCNT||1||Solution mixing||1.6710-2||-||Lee et al., 2011|
|Epoxy||MWCNT||8||3-roll mill||2.3104||0.0117||Iosif et al., 2009|
|Epoxy||SDS-MWCNTs||0.5||Bulk mixing||2.510-7||-||Santos et al., 2008|
|Nafion||SWCNTs||18||Solution mixing||3.2103||-||Landi et al., 2002|
4. Smart, multifunctional applications of carbon nanotube composites
CNT-based polymer composites have found numerous multifunctional applications owing to their capability to serve as reinforcing, lightweighting agents and a material platform for electrostatic discharging, electromagnetic interference shielding, radar absorbing, mechanical/chemical sensing, energy harvesting, and flame retardation. Smart applications can be categorized into sensing and actuation, and this chapter will primary focus on the review of research on electromechanical sensing using CNT-based polymer composites. The studies on sensors and actuators based on CNTs and their composites up to 2007 are well summarized by Li et al. (Li et al., 2008), and this chapter primarily presents more recent studies.
4.1. CNT Nanocomposites for electromechanical sensing
Electromechanical sensing and structural health monitoring typically utilize the piezoresistive behavior of the electrically conductive network formed by CNTs in polymer matrices, that is, the behavior characterized by a change in resistivity with respect to the structural deformation incurred by an external load. For example, when a CNT nanocomposite is subjected to a tensile load, the percolated CNT network is disrupted, resulting in an increase in resistivity. The variation in resistivity under a load is attributed to the variation in contact configurations and tunnelling distances among the contacting CNTs upon nanocomposite deformation.
Initial studies on piezoresistivity of conductive CNT network involved free-standing CNT films or sheets, also known as “buckypapers.” CNT buckypapers are typically made by filtration, similar to the papermaking process, where the CNTs are uniformly dispersed in a solvent, usually with the aid of surfactants, and subsequently passed through a filtering paper on which the CNTs are eventually deposited, dried, and detached. The CNT sheets were bonded to the surfaces of various substrates, including brass (Li
It has been reported that CNTs can be added to various materials, including general-purpose thermoplastics and thermosets, specialty polymers, such as polyvinylidene fluoride (PVDF) and shape memory polymers, elastomers, and concrete, and utilize the piezoresistivity of the nanocomposites for strain or pressure sensing.
4.1.1. Thermoplastic-based nanocomposites
The research group at the University of Cincinnati (Kang et al., 2006) reported comprehensive research work on strain sensing using buckypapers and SWCNT-polymethylmethacrylate(PMMA) composites. Fig. 12(a) shows the strain response of a SWCNT buckypaper sensor, which shows higher sensitivity in the linear bending range. However, it shows saturated strain behavior above 500 microstrains, which is probably attributed to the slippage among CNT bundles due to the weak van der Waals interactions at nanotube interfaces. When the sensor is compressed, the individual CNTs do not slip as much as compared to the tension case, resulting in the lack of saturation. Fig. 12(b) shows the strain response of composite sensor at varying CNT loadings. Although the composite strain sensors show lower sensitivities than buckypaper, they show linear symmetric strain response trends in both compression and tension. The interfacial bonding between CNTs and the polymer reduces slip and effectively increases the strain in the sensor.
Pham et al. (Pham et al., 2008) reported the development of conductive, MWCNT-filled, polymer composite films that can be used as strain sensors with tailored sensitivity. The electrical resistance of MWCNT-PMMA composite films subjected to tensile strains was measured, and the potential applications of the films as strain sensors with a broad range of tunable sensitivity were investigated. The surface resistivity of the films was observed to increase with increasing tensile strain, which is due to the reduction in conductive network density and increase in inter-tube distances induced by applied strains. The highest sensitivity achieved in this study was almost an order of magnitude greater than conventional resistance strain gages (Fig. 13). A semi-empirical model, based on the percolation theory, was developed to identify the relationship between applied strain and sensitivity factor (Fig. 14). Not only can the sensitivity be tailored over a broad, but also it can be increased significantly be having the conductive filler content approach the percolation threshold.
Zhang et al. (Zhang et al., 2006) presented a study on MWCNT-polycarbonate(PC) composites as multifunctional strain sensors, where a 5 wt.% composite showed instantaneous electrical resistance response to linear and sinusoidal dynamic strain inputs and a sensitivity of ~3.5 times that of a typical strain gage. Billoti
Abraham et al. (Abraham et al., 2008) reported the development and characterization of a CNT-PMMA nanocomposite flexible strain sensor for wearable health monitoring applications. These strain sensors can be used to measure the respiration rhythm which is a vital signal required in health monitoring. A number of strain sensor prototypes with different CNT compositions have been fabricated and their characteristics for both static as well as dynamic strain have been measured. Bautista-Quijanoa
CNTs were added to a piezoelectric polymer, PVDF, to for various smart applications, including strain sensing. Deshmukh et al. (Deshmukh et al., 2009) presented an experimental evidence of the creation of an electrostrictive response in PVDF by addition of small quantities of CNTs. It was demonstrated that the piezoelectric response of nanocomposites can be dramatically enhanced through addition of conductive nanoparticles such as CNTs without additional weight penalties. Most importantly, these improvements were achieved at much lower actuation voltages and were accompanied by an increase in both mechanical and dielectric properties. In the work by Kim et al. (Kim et al., 2008), CNTs were included in a PVDF matrix to enhance the properties of PVDF. The CNT-PVDF composite was fabricated by solvent evaporation and melt pressing. The inclusion of CNT allowed the dielectric properties of PVDF to be adjusted such that lower poling voltages can be used to induce a permanent piezoelectric effect in the composite. The CNT-PVDF composites were mounted on the surface of a cantilever beam to compare the voltage generation of the composite against homogeneous PVDF thin films.
4.1.2. Thermoset-based nanocomposites
The primary types of thermosets used as the matrices for strain sensing nanocomposites include epoxy, vinyl ester, and polyimide, among which epoxies are most popular. In the work by Wichmann et al. (Wichmann et al., 2009), electrically conductive epoxy based nanocomposites based on MWCNTs and carbon black were investigated concerning their potential for strain sensing applications with electrical conductivity methods. It was found that the nanocomposites exhibited a distinct resistance vs. strain behavior in the regime of elastic deformation, which is in good agreement with prevalent theories about charge carrier transport mechanisms in isolator/conductor composites. Applying an analytical model, it was shown that the piezoresistivity of nanocomposites may contribute valuable information about the conductive network structure and charge carrier transport mechanisms occurring in the nanocomposites. The authors also developed a direction-sensitive bending strain sensor consisting of a single block of MWCNT-epoxy composite by generating a gradient in electrical conductivity throughout the material (Wichmann et al., 2008).
Zhang et al. (Zhang et al., 2007) demonstrated a simple, effective and real-time diagnostic, and repair technique featuring MWCNTs that are infiltrated into epoxy. It was shown that by monitoring volume and through-thickness resistances, one can determine the extent and propagation of fatigue-induced damage such as crack and delamination growth in the vicinity of stress concentrations (Fig. 15). The conductive nanotube network also provides opportunities to repair damage by enabling fast heating of the crack interfaces; the authors show up to 70% recovery of the strength of the undamaged composite.
Quasi-static and dynamic strain sensing of CNT-epoxy composites was studied by Anand and Mahapatra (Anand & Mahapatra, 2009), and de la Vega,
4.1.3. Elastomer-based nanocomposites
Hwang et al. (Hwang et al., 2011) fabricated a piezoresistive composite using MWCNTs as a conductive filler and polydimethylsiloxane (PDMS) as a polymer matrix, which operated in the extremely small pressure range required for finger-sensing. To achieve a homogeneous dispersion of MWCNTs in PDMS, the MWCNTs were modified by a polymer wrapping method using poly(3-hexylthiophene) (P3HT). The percolation threshold of the composites was significantly lowered by the presence of P3HT. The electrical conductivity and piezoresistive sensitivity of the composite were found to strongly depend on the P3HT concentration. The well-dispersed P3HT-MWCNT/PDMS composite showed good piezoresistive characteristics in the 0–0.12 MPa pressure range.
Wang et al. (Wang et al., 2010) studied the piezoresistivity of a multi-walled carbon nanotube filled silicone rubber composite under uniaxial pressure. The experimental results showed that the active carboxyl radical on multi-walled carbon nanotubes can effectively improve the homogeneous distribution and alignment of conductive paths in the composite. As a result, the composite presented positive piezoresistivity with improved sensitivity and sensing linearity for pressure, both of which are key parameters for sensor applications. Elastomeric composites based on ethylene-propylene-diene-monomer (EPDM) filled with MWCNTs showed improved mechanical properties as compared to the pure EPDM matrix (Ciselli et al., 2010). A linear relation was found between conductivity and deformations up to 10% strain, which means that such materials could be used for applications such as strain or pressure sensors. Cyclic experiments were conducted to establish whether the linear relation was reversible, which is an important requirement for sensor materials.
High-elasticity CNT-methylvinyl silicone rubber (VMQ) nanocomposites with a high sensitivity and linear piezoresistive behavior was fabricated by dispersing conductive MWCNTs with different aspect ratios, AR = 50 and 500, into rubber matrix homogeneously (Dang et al., 2008). It was found that the percolation threshold of the nanocomposites containing AR = 50 MWCNTs was significantly lower than those containing AR = 500 MWCNTs. Extremely sensitive positive-pressure coefficient effect of the resistance and excellent cyclic compression under low pressure were also observed in the MWCNT-VMQ nanocomposites with AR = 50 MWCNTs at relatively low loadings.
4.2. CNT-based multiscale hybrid composite for electromechanical sensing
Multiscale hybrid composites (MHCs) are defined as composites consisting of at least three constituents having more than two different length scales. The most common type consists of the resin (macro), continuous (unidirectional or woven) fiber fabric (micro), and nanoparticles (nano) (Fig. 16). Conventional continuous fiber-reinforced plastics (FRPs) are characterized by extremely high in-plane modulus and stiffness (fiber-dominated) and poor through-thickness properties (matrix-dominated). In MHCs, high-performance nanomaterials are added to improve the through-thickness properties and, at the same time, to impart multifunctionalities to the composites.
Research on structural health monitoring of MHCs using the piezoresistivity of the percolated network of CNTs has been pioneered by the University of Delaware. A typical MHC manufacturing process involved dispersion of CNTs in the resin using a three-roll mill, followed by composite fabrication using vacuum-assisted resin transfer molding. The MHCs thus obtained were tested under various loading conditions to
An alternative way to incorporate CNTs in FRPs is to surface treat or coat the fibers with CNTs, instead of dispersing them in the resin. Specific methods include dipping the fibers into a CNT solution (Gao et al., 2010), aid of coupling agents (Sureeyatanapas & Young, 2009), lay-by-layer deposition (Loh et al., 2009), and direct growth of CNTs on the fibers using electrophoresis (Bekyarova et al., 2007). Another unique method is to embed continuous CNT fibers (Alexopoulos et al., 2010) or threads (Abot et al., 2010) in FRPs for large-area strain sensing.
CNTs have made inroads into multifunctional, smart applications, particularly strain sensing for structural health monitoring. A vast number of studies have focused on tailoring the mechanical and electrical properties of CNT-based nanocomposites by controlling CNT dispersion, orientation, and CNT-matrix interface at the nanoscale. The insights gained from the electromechanical behavior of CNT nanocomposites have open up a new field in structural health monitoring of multiscale hybrid composites. Although fundamental studies on processing-structure-property relationship in CNT nanocomposites need to be continued, allied efforts will need to be devoted to large-area strain mapping, cumulative stress/strain tracking, damage detection and life prediction algorithms, and data acquisition and analysis to fully utilize the smart sensing and actuation capabilities of CNT nanocomposites.
This research was supported by Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science and Technology (Grant No. 2009-0070548).
Abdalla M. Dean D. Theodore M. Fielding J. Nyairo E. Price G. 2010 Magnetically processed carbon nanotube/epoxy nanocomposites: Morphology, thermal, and mechanical properties. , 51 7 1614 1620, 0032-3861
Abot J. L. Song Y. Vatsavaya M. S. Medikonda S. Kier Z. Jayasinghe C. Rooy N. Shanov V. N. Schulz M. J. 2010 Delamination detection with carbon nanotube thread in self-sensing composite materials. , 70 1113 1119, 0266-3538
Abraham J. K. Aryasomayajula L. Whitchurch A. Varadan V. K. 2008 Carbon nanotube strain sensors for wearable patient monitoring applications, , 6931 0027-7786X
Ajayan P. Stephen O. Colliex C. Trauth D. 1994 Aligned Carbon Nanotube Arrays Formed by Cutting a Polymer Resin-Nanotube Composite,, 265 5176 1212 1214, 0036-8075
Alexopoulos N. D. Bartholome C. Poulin P. Marioli-Riga Z. 2010 Structural health monitoring of glass fiber reinforced composites using embedded carbon nanotube (CNT) fibers. , 70 260 271, 0266-3538
Allaoui A. Bai S. Cheng H. Bai J. 2002 Mechanical and electrical properties of a MWNT/epoxy composite. , 62 15 1993 1998, 0266-3538
Anand S. V. Mahapatra D. R. 2009 Quasi-static and dynamic strain sensing using carbon nanotube/epoxy nanocomposite thin films. , 1845013, 0964-1726
Awasthi K. Kamalakaran R. Singh A. Srivastava O. 2004 Ball-milled carbon and hydrogen storage. , 27 4 425 432, 0360-3199
Bal S. Samal S. 2007 Carbon Nanotube Reinforced Polymer Composite-A State of The Art., 30 4 379 386, 0250-4707
Bautista-Quijanoa J. R. Avilésa F. Aguilara J. O. Tapia A. 2010 Strain sensing capabilities of a piezoresistive MWCNT-polysulfone film. A, 159 135 140, 0924-4247
Bekyarova E. Thostenson E. T. Yu A. Kim H. Gao J. Tang J. Hahn H. T. Chou T.W. Itkis M. E. Haddon R. C. 2007 Multiscale carbon nanotube-carbon fiber reinforcement for advanced epoxy composites., 23 3970 3974, 0743-7463
Bhattachacharyya A. Sreekumar T. Liu T. Kumar S. Ericson L. Hauge H. Smalley R. 2003Crystallization and orientation studies in polypropylene/single wall carbon nanotube composite. , 44 8 2373 2377, 0032-3861
Baughman R. Zakhidov A. de Heer W. 2002Carbon Nanotubes, The Route Toward Applications. , 297 5582 787 792, 0036-8075
Bauhofer W. Kovacs J. 2009 A review and analysis of electrical percolation in carbon nanotube polymer composites, , 69 10 1486 1498 0266-3538
Bilotti E. Zhang R. Deng H. Baxendale M. Peijs T. 2010 Fabrication and property prediction of conductive and strain sensing TPU/CNT nanocomposite fibres, , 20 9449 9455, 0959-9428
Boger L. Wichmann M. H. G. Meyer L. O. Schulte K. 2008 Load and health monitoring in glass fibre reinforced composites with an electrically conductive nanocomposite epoxy matrix. , 68 1886 1894, 0266-3538
Camponeschi E. Vance R. Al-Haik M. Garmestani H. Tannenbaum R. 2007 Properties of nanotube-polymer composites aligned in a magnetic field, , 45 10 2037 2046, 0032-3861
Chang T. Kisliuk A. Rhodes S. Brittain W. Sokolov A. 2006 Conductivity and mechanical properties of well-dispersed single-wall carbon nanotube/polystyrene composite. , 47 22 7740 7746, 0032-3861
Cheng F. Imin P. Maunders C. Botton G. Adronov A. 2008Soluble, discrete supramolecular complexes of single-walled carbon nanotubes with fluorene-based conjugated polymers. , 41 7 2304 2308, 0024-9297
Ci L. Suhr J. Pushparaj V. Zhang X. Ajayan P. 2008 Continuous Carbon Nanotube Reinforced Composites. , 8 9 2762 2766 1530-6984
Ciselli P. Lu L. Busfield J. J. C. Peijs T. 2010 Piezoresistive polymer composites based on EPDM and MWNTs for strain sensing applications. , 14 1618-7229
Coleman J. Khan U. Blau W. Gun’ko Y. 2006 Small but Strong: A Review of The Mechanical Properties of Carbon Nanotube-Polymer Composites. , 44 9 1624 1652, 0008-6223
Dang Z. M. Jiang M.J. Xie D. Yao S.H. Zhang L. Q. Bai J. 2008 Supersensitive linear piezoresistive property in carbon nanotubes/silicone rubber nanocomposites. ., 10424114, 0021-8979
de la Vega A. Kinloch I. A. Young R. J. Bauhofer W. Schulte K. 2011 Simultaneous global and local strain sensing in SWCNT-epoxy composites by Raman and impedance spectroscopy. , 71 160 166, 0266-3538
Deshmukh S. Ounaies Z. Krishnamoorti R. 2009 Polymer nanocomposites as electrostrictive materials, , 7289 0027-7786X
Dresselhaus M. 1997 Future Directions in Carbon Science. , 27 1 1 34, 1531-7331
Dresselhaus M. Dresselhaus G. Charlier J. Hernández E. 2004Electronic, thermal and mechanical properties of carbon nanotubes. , 15 362 2065 2098, 0136-4503X
Gao L. Thostenson E. T. Zhang Z. Chou T.W. 2009 Sensing of damage mechanisms in fiber-reinforced composites under cyclic loading using carbon nanotubes. , 19 123 130, 0161-6301X
Gao S. L. Zhuang R.C. Zhang J. Liu J.W. Mader E. 2010 Glass fibers with carbon nanotube networks as multifunctional sensors. , 20 1885 1893, 0161-6301X
Gorrasi J. Sarno M. Di Bartolomeo A. Sannino D. Ciambelli P. Vittoria V. 2007 Incorporation of carbon nanotubes into polyethylene by high energy ball milling: morphology and physical properties. , 45 5 597 606, 0887-6266
Haluska M. Hulman M. Hirscher M. Becher M. Roth S. Stepanek I. Bernier P. 2001 Hydrogen storage in mechanically treated single wall carbon nanotubes. , 591 603 608.
Hernandez J. Garcia-Gutierrez M. Nogalas A. Rueda D. Kwiatkowska M. Szymczyk A. Roslaniec Z. Concheso A. Guinea I. Ezquerra T. 2009Influence of preparation procedure on the conductivity and transparency of SWCNT-polymer composites. , 69 11-12 1867 1872, 0266-3538
Hwang J. Jang J. Hong K. Kim K. N. Han J. H. Shin K. Park C. E. 2011Poly(3-hexylthiophene) wrapped carbon nanotube/poly(dimethylsiloxane) composites for use in finger-sensing piezoresistive pressure sensors. , 49 106 110, 0008-6223
Iosif D. Rosca Suong. V. Hoa 2009 Highly conductive multiwall carbon nanotube and epoxy composites produced by three-roll milling. , 47 8 1958 1968, 0008-6223
Jia Z. Wang Z. Liang J. Wei B. Wu D. 1999 Production of short multi-walled carbon nanotubes. , 37 37 6 903 906. 0008-6223
Jiang X. Bin Y. Matsuo M. 2005 Electrical and mechanical properties of polyimide-carbon nanotubes composites fabricated by in situ polymerization. , 46 18 7418 7424, 0032-3861
Jin Y. Yuan F. 2003 Simulation of Elastic Properties of Single-Walled Carbon Nanotubes. , 63 11 1507 1515, 0266-3538
Kang I. Yun Y. H. Kim J. H. Lee J. W. Gollapudi R. Subramaniam S. Narasimhadevara S. Hurd D. Kirikera G. R. Shanov V. Schulz M. J. Shi D. Boerio J. Mall S. Ruggles-Wren M. 2006 Introduction to carbon nanotube and nanofiber smart materials. , 37 382 394, 1359-8368
Kang J. H. Park C. Scholl J. A. Brazin A. H. Holloway N. M. High J. W. Lowther S. E. Harrison J. S. 2009 Piezoresistive characteristics of single wall carbon nanotube/polyimide nanocomposites. , 47 994 1003, 0887-6266
Kim H. Kim K. Lee S. Joo J. Yoon H. Cho S. Lyu S. Lee C. 2004 Charge transport properties of composites of multiwalled carbon nanotube with metal catalyst and polymer: application to electromagnetic interference shielding. , 4 6 577 580, 1567-1739
Kim J. Loh K. J. Lynch J. P. 2008 Piezoelectric polymeric thin films tuned by carbon nanotube fillers, , 6932 0027-7786X
Kim K. J. Yu W. R. Lee J. S. Gao L. Thostenson E. T. Chou T. W. Byun J.H. 2010 Damage characterization of 3D braided composites using carbon nanotube-based in situ sensing, , 41 1531 1537, 0135-9835X
Ko F. Gogotsi Y. Ali A. Naguib N. Ye H. Yang G. Li C. Willis P. 2003 Electrospinning of Continuous Carbon Nanofiber Yarns. Adv. Mater., 15 14 1161 1165, 0935-9648
Koerner H. Liu W. Alexander M. Mirau P. Dowty H. Vaia R. 2005Deformation-morphology correlations in electrically conductive CNT-thermoplastic polyurethane nanocomposites. , 46 12 4405 4420 0032-3861
Krause B. Pötschke P. Häuser L. 2009 Influence of small scale melt mixing conditions on electrical resistivity of carbon nanotube-polyamide composites. , 69 10 1505 1515, 0266-3538
Landi B. Raffaelle R. Heben M. Alleman J. Van Derveer W. Gennett T. 2002 Single wall carbon nanotube-nafion composite actuators. , 2 11 1329 1332, 1530-6984
Lee J. Rhee K. Park S. Silane modification of carbon nanotubes and its effects on the material properties of carbon/CNT/epoxy three-phase composites. , 42 42 5 478 EOF 483 EOF, 0135-9835X
Li C. Thostenson E. T. Chou T. Chou W. 2008 Sensors and actuators based on carbon nanotubes and their composites: A review. , 68 1227 1249, 0266-3538
Li X. Levy C. Elaadil L. 2008 Multiwalled carbon nanotube film for strain sensing., 1945501, 0957-4484
Li Z. Dharap P. Nagarajaiah S. Barrera E. V. Kim J. D. 2008 Carbon nanotube film sensors. , 16 7 640 643, 0935-9648
Loh K. J. Hou T.C. Lynch J. P. Kotov N. A. 2009 Carbon nanotube sensing skins for spatial strain and impact damage identification. , 28 9 25, 0195-9298
Lu K. Lago R. Chen Y. Green M. Harris P. Tsang S. 1996 Mechanical damage of carbon nanotubes by ultrasound. , 34 6 814 816 0008-6223
Ma P. Siddiquia N. Maromb G. Kim J. 2010Dispersion snd Functionalization of Carbon Nanotubes for Polymer-Based Nanocomposites: A Review. , 41 10 1345 1367, 0135-9835X
Martin C. Sandler J. Windle A. Schwarz M. Bauhofer W. Schulte K. Shaffer M. 2005 Electric field-induced aligned multi-wall carbon nanotube networks in epoxy composites. , 46 3 877 886 0032-3861
Mičušík M. Omastová M. Krupa I. Prokeš J. Pissis P. Logakis Pandis. C. Pötschke P. Piontek J. 2009A comparative study on the electrical and mechanical behaviour of multi-walled carbon nanotube composites prepared by diluting a masterbatch with various types of polypropylene. , 113 4 2536 2551, 00218995
Narayan C. Yayong L. Kaikun Y. Weiqun P. Spandan M. Howard W. 2009Single-Walled Carbon Nanotube/Poly(methyl methacrylate) Composites for Electromagnetic Interference Shielding, , 49 8 1627 1634 0032-3888
Nativ-Roth E. Shvartzman-Cohen R. Bounioux C. Florent M. Zhang D. Szleifer I. Yerushalmi-Rozen R. 2007Physical adsorption of block copolymers to SWNT and MWNT: a nonwraping mechanism. , 40 10 3676 3685, 0024-9297
Oh J. Ahn K. Hong J. 2010 Dispersion of entangled carbon nanotube by melt extrusion. , 22 2 89 94 0122-6119X
Peng H. Sun X. 2009 Highly aligned carbon nanotube/polymer composites with much improved electrical conductivities. , 471 1-3 103 105, 0009-2614
Pham G. T. Park Y. B. Liang Z. Zhang C. Wang B. 2008 Processing and modeling of conductive thermoplastic/carbon nanotube films for strain sensing. , 39 209 216, 1359-8368
Pötschke P. Fornes T. Paul D. 2002Rheological behaviour of multiwalled carbon nanotubes/polycarbonate composites. , 43 11 3247 3255, 0032-3861
Ramasubramaniam R. Chen J. Liu H. 2003 Homogeneous carbon nanotube/ polymer composites for electrical applications, 83 14 2928 2930, 0003-6951
Sahoo N. Ranab S. Cho J. Li L. Chan S. 2010 Polymer nanocomposites based on functionalized carbon nanotubes. , 35 7 837 867, 0079-6700
Salalha W. Dror Y. Khalfin R. Cohen Y. Yarin A. Zussman E. 2004 Single-Walled Carbon Nanotubes Embedded in Oriented Polymeric Nanofibers by Electrospinning. , 20 20 9852 9855, 0743-7463
Sandler J. Kirk J. Kinloch I. Shaffer M. Windle A. 2003 Ultra-low electrical percolation threshold in carbon-nanotube-epoxy composites. , 44 19 5893 5899, 0032-3861
Santos A. Leite T. Furtado C. Welter C. Pardini L. Silva G. 2008Morphology, thermal expansion, and electrical conductivity of multiwalled carbon nanotube/epoxy composites. ., 108 2 979 986, 0021-8995
Seifert G. Kohler T. Frauenheim T. 2000 Molecular wires, solenoids, and capacitors by sidewall functionalization of carbon nanotubes. , 77 9 1313 1315 0003-6951
Shelimova K. Esenalieva R. Rinzlera A. Huffman C. Smalley R. 1998Purification of single-wall carbon nanotubes by ultrasonically assisted filtration. , 282 5-6 429 434, 0009-2614
Spitalskya Z. Tasisb D. Papagelis K. Galiotis C. 2010Carbon nanotube-polymer composites: Chemistry, processing, mechanical and electrical properties. , 35 3 357 401, 0079-6700
Stevens J. Huang A. Peng H. Chiang I. Khabashesku V. Margrave J. 2003Sidewall amino-functionalization of SWNTs through fluorination and subsequent reactions with terminal diamines. , 3 3 331 336, 1530-6984
Sureeyatanapas P. Young R. J. 2009 SWNT composite coatings as a strain sensor on glass fibres in model epoxy composites. , 69 1547 1552, 0266-3538
Thess A. Lee R. Nikolaev P. Dai H. Petit P. Robert J. Xu C. Lee H. Kim S. Rinzler A. Colbert D. Scuseria G. Tomanek D. Fischer J. Smalley R. 1996 Crystalline ropes of metallic carbon nanotubes. , 273 5274 483 488, 0036-8075
Thostenson E. Chou T. 2002Aligned multi-walled carbon nanotube-reinforced composites: processing and mechanical characterization , 35 16 L77 L80 0022-3727
Thostenson E. T. Chou T. W. 2006 Processing-structure-multi-functional property relationship in carbon nanotube/epoxy composites. , 44 14 3022 3029. 0008-6223
Thostenson E. T. Chou T. W. 2006 Carbon nanotube networks: sensing of distributed strain and damage for life prediction and self healing. , 18 2837 2841, 0935-9648
Thostenson E. T. Ziaee S. Chou T.W. 2009 Processing and electrical properties of carbon nanotube/vinyl ester nanocomposites. , 69 801 804, 0266-3538
Vemuru S. M. Wahi R. Nagarajaiah S. Ajayan P. M. 2009 Strain sensing using a multiwalled carbon nanotube film. , 44 555 562, 0309-3247
Vigolo B. Pe´nicaud A. Coulon C. Sauder C. Pailler R. Journet C. Bernier P. Poulin P. 2000 Macroscopic Fibers and Ribbons of Oriented Carbon Nanotubes. , 290 5495 1331 1334, 0036-8075
Viswanathan V. Laha T. Balani K. Agarwal A. Seal S. 2006 Challenges and advances in nanocomposite processing techniques. , 54 5-6 121 285, 0092-7796X
Wang Q. Dai J. Li W. Wei Z. Jiang J. 2008 The effects of CNT alignment on electrical conductivity and mechanical properties of SWNT/epoxy nanocomposites. , 68 7-8 2208 2213, 0266-3538
Wang P. Geng S. Ding T. 2010 Effects of carboxyl radical on electrical resistance of multi-walled carbon nanotube filled silicone rubber composite under pressure. , 70 1571 1573, 0266-3538
Wichmann M. H. G. Buschhorn S. T. Boger L. Adelung R. Schulte K. 2008 Direction sensitive bending sensors based on multi-wall carbon nanotube/epoxy nanocomposites. , 19475503, 0957-4484
Wichmann M. H. G. Buschhorn S. T. Gehrmann J. Schulte K. 2009 Piezoresistive response of epoxy composites with carbon nanoparticles under tensile load. , 80245437, 1098-0121
Yuen S. Ma C. Lin Y. Kuan H. 2007 Preparation, morphology and properties of acid andamine modified multiwalled carbon nanotube/polyimide composite. , 67 11-12 2564 2573, 0266-3538
Zhang M. Atkinson K. Baughman R. 2004 Multifunctional Carbon Nanotube Yarns by Downsizing an Ancient Technology. , 306 1358 1361 0036-8075
Zhang Q. Rastogi S. Chen D. Lippits D. Lemstra P. 2006 Low percolation threshold in single-walled carbon nanotube/high density polyethylene composites prepared by melt processing technique. , 44 4 778 785, 0008-6223
Zhang W. Suhr J. Koratkar N. 2006 Carbon nanotube/polycarbonate composites as multifunctional strain sensors., 6 960 964, 1533-4880
Zhang W. Sakalkar V. Koratkar N. 2007 In situ health monitoring and repair in composites using carbon nanotube additives. 91 133102 EOF, 0003-6951